Fabrication, Characterization, and Energetic Properties of Metallized Fibers Nicholas A. Clayton,† Keerti S. Kappagantula,‡ Michelle L. Pantoya,‡ Sharon C. Kettwich,*,† and Scott T. Iacono*,† †
Department of Chemistry and Chemistry Research Center, United States Air Force Academy, 2355 Fairchild Drive, Suite 2N225, USAF Academy, Colorado 80840, United States ‡ Department of Mechanical Engineering, Texas Tech University, Lubbock, Texas 79409, United States ABSTRACT: Polystyrene ﬁbers loaded with an energetic blend of nanoaluminum (n-Al) and perﬂuoropolyether (PFPE) were successfully fabricated via electrospinning producing nanothermite fabrics. Fibers were generated with loadings up to 17 wt % n-Al/PFPE incorporated into the ﬁber. Microscopy analysis by SEM and TEM conﬁrm a uniform dispersion of PFPE treated n-Al on the outside and inside of the ﬁbers. Metallized ﬁbers were thermally active upon immediate ignition from a controlled ﬂame source. Thermal analysis by diﬀerential scanning calorimetry (DSC) found no change in glass transition temperature when comparing pure polystyrene ﬁbers with ﬁbers loaded up to 17 wt % n-Al/PFPE. Thermal gravimetric analysis (TGA) revealed a shift in decomposition temperatures to lower onsets upon increased loadings of n-Al/PFPE blends, consistent with previous studies. Flame propagation studies conﬁrmed that the metallized ﬁbers are pryolants. These metallized ﬁbers are a recent development in metastable intermolecular composites (MICs) and details of their synthesis, characterization, and thermal properties are presented. KEYWORDS: nanothermite, pyrolant, energetic material, electrospinning, nanoparticles
challenges associated with melt casting or ball milling of nanometallized propellants, for example, pre- or post-burning aggregation, can be mitigated. The technique of electrospinning has been around since the 1930s, but the mechanism behind the spinning was vaguely understood until the 1990s.17 For the most part, electrospinning is simple and versatile whereby ultrathin polymer composite and ceramic-based ﬁbers can easily be produced. In general, the morphology and diameter of electrospun ﬁbers are dependent on the intrinsic physical properties of the precursor solution (concentration, viscosity, and electrical conductivity) and the operating conditions (strength of the applied electric ﬁeld, distance between spinneret and substrate, and ﬂow rate of precursor solution).17 We have recently reported the fabrication of metallized energetic epoxide-based composites.15 An energetic blend of nanoaluminum (n-Al) coated with perﬂuoropolyether (PFPE) (Figure 1) was successfully loaded into a partially cured epoxide and allowed to fully cure. The resulting rigid material did not degrease beyond its glass transition temperature, is indeﬁnitely shelf-stable, and can be post-machined (drilled, milled, or Special Issue: Applications of Hierarchical Polymer Materials from Nano to Macro Received: October 17, 2013 Accepted: December 17, 2013 Published: December 31, 2013 6049
values.25 Initially, our attempts failed to eﬀectively electrospin Teﬂon AF dissolved in a variety of ﬂuorinated solvents (hexaﬂuorobenzene, Asahiklin AK-225, 3M Fluorinert FC75). It has been demonstrated that room temperature ionic liquids such as 1-butyl-3-methylimidazolium hexaﬂuorophosphate (BMIM-PF6) can be added to the precursor suspension with a similar partially ﬂuorinated, amorphous polymer in low amounts (>1.5 wt %) to make the suspension more electrospinnable.26 BMIM-PF6 was added to a suspension of Teﬂon AF® yet generation of ﬁbers via electrospinning was still unsuccessful. Teﬂon AF® has successfully been electrospun by implementing a coaxial electrospinning technique where an electrospinnable polymer is used as a so called guiding material to facilitate spinning.25,27,28 In one case, poly(vinylidene ﬂuoride) (PVDF) was used as a guiding material, but only 1 wt % Teﬂon AF® was successfully incorporated into ﬁbers.25 Instead of attempting coaxial electrospinning, polystyrene (PS) was chosen as the precursor polymer to be electrospun into ﬁbers. Lacking ﬂuorocarbon substitution, PS has a higher dielectric constant and has been employed in the commercial manufacture of electrospun ﬁbers; it was determined PS could serve as a suitable matrix material for this model study. We also attempted to electrospin ﬁbers loaded with n-Al only (no PFPE), but the metal particles would not remain as a stable suspension in PS/DMF. Similarly, when n-Al and PFPE were added to the PS/DMF solution independently (i.e., were not pre-coated), the constituents of the suspension would also separate. Polystyrene ﬁbers loaded with a uniform distribution of PFPE coated n-Al ﬁbers can only be produced when the precoating method is followed to prevent aggregation/agglomeration of the particles. The results are pictorially summarized in Figure 1; suspension separation was observed by eye; however, when photographed, the pictures failed to produce evident contrast. By not pre-coating the n-Al with PFPE, this causes separation of the suspension, clogging the syringe needle, and ultimately resulting in the inability to electrospin uniform metallized ﬁbers. The requirement of pre-coating the n-Al with the PFPE to make the particles miscible with the matrix was also observed when n-Al/PFPE blends were incorporated into epoxide matrices.15 Fiber diameters were determined via SEM and representative diameters for a range of ﬁber loadings are listed in Table 1 and SEM images are shown in Figure 2. As expected, the pure PS ﬁbers appear to have a smooth and regular surface morphology. Pure PS nanometer-sized ﬁbers were consistently achieved; however, upon loading with n-Al/PFPE, microﬁbers up to 5400 nm diameter were repeatedly achieved with no apparent correlation with wt% loading. A larger variation in diameter was observed for the 17 wt % n-Al/PFPE formulated ﬁbers (1900− 7900 nm) whereas electrospinning pure PS consistently produced ﬁbers 350 °C into volatile aromatic compounds producing char yields
Fabrication, characterization, and energetic properties of metallized fibers.
Polystyrene fibers loaded with an energetic blend of nanoaluminum (n-Al) and perfluoropolyether (PFPE) were successfully fabricated via electrospinnin...